Impact of Metal-Ion Dependence on the Porous and Electronic Properties of TCNQ-Dianion-Based Porous Coordination Polymers
Satoru Shimomura; Nobuhiro Yanai; Ryotaro Matsuda; Susumu Kitagawa; Inorganic Chemistry 50 (2011) 172–177; doi:10.1021/ic1015498

data_4324107
_publ_contact_author_address
;
 Department of Synthetic Chemistry 
 and Biological Chemistry, 
 Graduate School of Engineering, 
 Kyoto University, 
 Katsura, Kyoto 615-8510, Japan 
;
_publ_contact_author_email       kitagawa@sbchem.kyoto-u.ac.jp
_publ_contact_author_fax         +81-75-383-2732
_publ_contact_author_name        'Susumu Kitagawa'
_publ_contact_author_phone       +81-75-383-2733
_publ_section_title
;
 Impact of Metal-Ion Dependence on the Porous and Electronic Properties of
 TCNQ-Dianion-Based Porous Coordination Polymers
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              172
_journal_page_last               177
_journal_paper_doi               10.1021/ic1015498
_journal_volume                  50
_journal_year                    2011
_chemical_formula_moiety         'C30 Co N6 O8 '
_chemical_formula_sum            'C30 Co N6 O8'
_chemical_formula_weight         631.30
_space_group_IT_number           130
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      130
_symmetry_space_group_name_Hall  '-P 4a 2ac'
_symmetry_space_group_name_H-M   'P 4/n c c :2'
_cell_angle_alpha                90.0000
_cell_angle_beta                 90.0000
_cell_angle_gamma                90.0000
_cell_formula_units_Z            8
_cell_length_a                   17.302(8)
_cell_length_b                   17.302(8)
_cell_length_c                   22.789(11)
_cell_measurement_reflns_used    10506
_cell_measurement_temperature    223.1
_cell_measurement_theta_max      29.9
_cell_measurement_theta_min      1.7
_cell_volume                     6822(6)
_computing_cell_refinement       CrystalClear
_computing_data_collection       CrystalClear
_computing_data_reduction        CrystalStructure
_computing_publication_material  'CrystalStructure 3.8'
_computing_structure_refinement  CRYSTALS
_computing_structure_solution    SIR2002
_diffrn_ambient_temperature      223.1
_diffrn_detector_area_resol_mean 7.31
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Rigaku Mercury'
_diffrn_measurement_method       \w
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71070
_diffrn_reflns_av_R_equivalents  0.128
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            23406
_diffrn_reflns_theta_full        25.04
_diffrn_reflns_theta_max         25.04
_exptl_absorpt_coefficient_mu    0.555
_exptl_absorpt_correction_T_max  0.895
_exptl_absorpt_correction_T_min  0.569
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Jacobson, R. (1998) Private communication'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.229
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             2504.00
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.20
_refine_diff_density_max         0.84
_refine_diff_density_min         -0.81
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.059
_refine_ls_number_parameters     186
_refine_ls_number_reflns         1895
_refine_ls_R_factor_gt           0.0869
_refine_ls_shift/su_max          0.0000
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details
;
    Chebychev polynomial with 3 parameters (Carruthers & Watkin, 1979)
    13.6593    6.1239    9.9787
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.1209
_reflns_number_gt                1128
_reflns_number_total             3015
_reflns_threshold_expression     F^2^>2.0\s(F^2^)
_cod_data_source_file            ic1015498_si_001_3.cif
_cod_data_source_block           '__091112_CoTb_as_1'
_cod_original_sg_symbol_H-M      'P 4/n c c'
_cod_original_formula_sum        'C30 Co N6 O8 '
_cod_database_code               4324107